properties of low density
Post on 10-Mar-2016
Embed Size (px)
DESCRIPTION`The effect of ethylene diamine-isophthalic acid on tensile properties, morphology properties, water absorption, and thermal properties of the low density polyethylene/eggshell powder composites were studied.
PROPERTIES OF LOW DENSITY POLYETHYLENE (LDPE) / EGGSHELL POWDER
(ESP) COMPOSITES: THE EFFECT OF ETHYLENE DIAMINE-ISOPTHALIC ACID
A.G. SUPRI & SITI SHUHADAH
Division of Polymer Engineering, School Of Material Engineering, Universiti Malaysia Perlis (Unimap), 02600 Jejawi, Perlis, Malaysia
`The effect of ethylene diamine-isophthalic acid on tensile properties, morphology properties, water absorption,
and thermal properties of the low density polyethylene/eggshell powder composites were studied. The both composites,
low density polyethylene/eggshell powder (LDPE/ESP) and low density polyethylene / modified eggshell powder
(LDPE/ESPM) composites were prepared with Z-Blade Mixer at 1800C and rotor speed of 50 rpm. The results indicate that
the addition of ethylene diamine-isophthalic acid increased the tensile strength, Youngs modulus, glass transition
temperature (Tg), melting temperature (Tm), and water absorption resistance but lower percentage of crystallinity and the
elongation at break of the LDPE/ESP composites. The micrographs of SEM showed that the eggshell powder was more
widely dispersed in the LDPE matrix with the addition of ethylene diamine-isophthalic acid as a coupling agent.
KEYWORDS: Low Density Polyethylene, Ethylene Diamine-Isophthalic Acid, Eggshell Powder
In recent decades, growing environmental awareness has resulted in renewed interest in the use of natural
materials for different applications. Increasingly more stringent environmental policies have forced industries such as the
automotive, packaging and construction industries to search for new materials that can substitute traditional composite
materials consisting of a plastic matrix and inorganic reinforcement [1-2].The incorporation of mineral fillers into
thermoplastics has been widely practiced in industry to extend them and to enhance certain properties. Fillers often
increase the performance of polymeric products.
The degree of improvement on the judicious choice of filler origin, particle size and shape, the fraction of filler,
and the surface treatment promoting interaction between the polymer matrix and filler . The addition of fillers to
polymers is a fast and cheap method to modify the properties of the base materials. For this reason, particulate filled
polymers have been, and are, a subject of increasing interest in both industry and research. In this way, strength, stiffness,
electrical and thermal conductivity, hardness and dimensional stability, among other properties can be tailored to the
required values. The modification of the interfacial and interphase properties of polymer composites is mainly carried out
in order to achieve a certain degree of compatibilization in the system.
As described before, there are two ways to improve mechanical properties through the use of filler: by changing
its particle size and by treating it with coupling agents . Scanning electron microscopy (SEM) is routinely used for
morphology investigation of polymer blends and composites. Sample surface is observable by the SEM method and the
elements of the structure can be identified. A study of the surface after fracture is a frequently used mode of sample
preparation in SEM study of polymer morphology . This article reports that an investigation on the mechanical
International Journal of General Engineering and Technology (IJGET) ISSN: 2278-9928 Vol.1, Issue 2 Nov 2012 9-18 IASET
10 A.G. Supri & Siti Shuhadah
properties, thermal properties, water absorption, and morphology of unmodified (ESP) and modified eggshells powder
(ESPM) into low density polyethylene / eggshell powder composites.
MATERIALS AND EXPERIMENTAL
Low density polyethylene (LDPE) grade L705 (MFI 7g/10 min and density 0.918 g/cm3) was obtained from
Polyolefins Company, Singapore. The eggshell was obtained from local market. Ethanol (C2H5OH), sodium hydroxyl
(NaOH), ethylene diamine, and isophthalic acid with Mr 166.14 were supplied from Sigma-Aldrich Chemie GmbH,
Preparation of Eggshell Powder
Eggshells were washed, dried and grinded. Eggshell was grinded to powder using the blender. Sieve was used to
obtain an average filer sizes of 63 m. Eggshell Powder was dried in vacuum oven at 800C till the constant weight is
occurred to make it free from moisture. After that the Eggshells Powder were examined using the X-ray fluorescene
spectrometer as shown in Table 1.
Treated the Eggshell Powder
Eggshell powder has been average sizes of 63 m was treated by using the sodium hydroxide (NaOH). The
eggshell powder was mixed with the solution of 10% NaOH. The eggshell powder was mixed with the solution and stirred
for 6 minutes at room temperature until two layers is formed. The upper layer is decanted and the deprotenized layer that
is precipitate is washed with distilled water. The wash precipitated sample is dried in the oven at 1050C till the constant
Modified the Eggshell Powder
Chemical modification of modified eggshell powder was carried out by adding ethylene diamine-isophthalic acid
and ethanol. The eggshell powder was dipped in an ethanol solution containing ethylene diamine-isophthalic acid (6% by
weight of ESP) at 48 hours at 500C. The eggshell powder then decanted and dried in an air oven at temperature of 700C for
The formulation of low density polyethylene/eggshell powder (LDPE/ESP) composites and low density polyethylene /modified eggshell powder (LDPE/ESPM) is given in Table 1. The Z-Blade mixer was set at temperature of
180C and a rotor speed of 50 rpm. Low density polyethylene was then charged into Z-blade mixer to start the melt mixing.
LDPE was preheated for 20 minutes in the mixing chamber. Next, eggshell powder (ESP) or modified eggshell powder
(ESPM) are added to the soften LDPE. The mixing process was allowed for another 5 minutes in order to obtain
homogeneous composites. The composites was discharged from the mixing chamber and pressed into thick round pieces.
The discharged composites were then allowed to cool.
Samples of LDPE/ESP and LDPE/ESPM composites were compressed via an electrical heated hydraulic press to produce the composites in plate form. The hot press machine was set at the temperature of 180C for both top and bottom
platen. Then, the composites were put into the mould, preheated for 8 minutes followed by compression for 4 minutes at
the same temperature and subsequently cooled under pressure for 4 minutes.
Properties of Low Density Polyethylene (Ldpe) / Eggshell Powder (ESP) 11 Composites: The Effect of Ethylene Diamine-Isopthalic Acid
Mechanical Properties Test
Tensile properties were determined according to ASTM D638 by using the Instron 5569. Dumb-bell shaped
specimens were conditioned at ambient temperature (25 + 3) 0C and relative humidity (30 + 2) % before testing. A cross
head speed of 50mm/min was used. The average of five samples was used during the test.
Scanning Electron Microscopy
Studies on morphology of the tensile fracture surface of LDPE/ESP composites and LDPE/ESPM composites were carried out using a scanning electron microscopy (SEM) using SEM, model JEOL JSM 6460LA. Surfaces of the
samples were coated with a thin palladium layer of about 12 m thickness using Auto Fine Coater, model JEOL JFC 1600.
Water Absorption Test Water absorption test was carried out according to ASTM standard D750-95.It involved total immersion of three samples in distilled water at room temperature. All the specimens were previously dried in an oven at 500C for 24 h and
stored in desiccators. The water absorption was determined by weighing the samples at regular interval. A Mettler balance
type AJ150 was used with a precision of + 1 mg. The percentage of water absorption (Mt) was calculated by:
Where Wd and WN are original dry and weight after exposure respectively. The average reading of three samples was
Differential Scanning Calorimetry Analysis
Thermal analysis measurements of selected system were performed using a Perkin Elmer DSC-7 analyzer.
Samples of about 4 mg were heated from 25 to 2500C using a nitrogen air flow of 50 ml/min and heating rate of
100C/min.The melting and crystallization behavior of selected composites also performed using a Perkin Elmer DSC-7
analyzer. The % crystallinity of composites was determined using the following relationship;
x 100% (2)
Where Hf and Hof are enthalpy of fusion of the composite and enthalpy of fusion of LDPE, respectively. The value for
H of (LDPE) is 293.6J/g
RESULTS AND DISCUSSION
Figure 1 shows the tensile strength of LDPE/ESP and LDPE/ESPM composites with different filler loading. It can
be seen that the tensile strength of the both composites decreases with increasing the filler loading. The decreases of tensile
strength were due to the poor adhesion of filler-matrix and agglomeration of filler particles. At similar filler load